Removal of dyes using agricultural waste as low-cost adsorbents: a review
- 26k Downloads
Color removal from wastewater has been a matter of concern, both in the aesthetic sense and health point of view. Color removal from textile effluents on a continuous industrial scale has been given much attention in the last few years, not only because of its potential toxicity, but also mainly due to its visibility problem. There have been various promising techniques for the removal of dyes from wastewater. However, the effectiveness of adsorption for dye removal from wastewater has made it an ideal alternative to other expensive treatment methods. In this review, an extensive list of sorbent literature has been compiled. The review evaluates different agricultural waste materials as low-cost adsorbents for the removal of dyes from wastewater. The review also outlines some of the fundamental principles of dye adsorption on to adsorbents.
KeywordsDyes Low-cost adsorbents Adsorption Wastewater treatment
Dyes are widely used in industries such as textiles, rubber, plastics, printing, leather, cosmetics, etc., to color their products. As a result, they generate a considerable amount of colored wastewater. There are more than 10,000 commercially available dyes with over 7 × 105 tonnes of dye stuff produced annually. It is estimated that 2 % of dyes produced annually is discharged in effluents from associated industries (Allen and Koumanova 2003). Among various industries, textile industry ranks first in usage of dyes for coloration of fiber. The total dye consumption of the textile industry worldwide is in excess of 107 kg/year and an estimated 90 % of this ends up on fabrics. Consequently, 1,000 tones/year or more of dyes are discharged into waste streams by the textile industry worldwide (Marc 1996). Discharge of dye-bearing wastewater into natural streams and rivers poses severe problems to the aquatic life, food web and causes damage to the aesthetic nature of the environment.
Dyes absorb and reflect sunlight entering water and so can interfere with the growth of bacteria and hinder photosynthesis in aquatic plants. The problems become graver due to the fact that the complex aromatic structures of the dyes render them ineffective in the presence of heat, light, microbes, and even oxidizing agents and degradation of the dyes become difficult (Pearce et al. 2003). Hence, these pose a serious threat to human health and water quality, thereby becoming a matter of vital concern. Keeping the essentiality of color removal, concerned industries are required to treat the dye-bearing effluents before dumping into the water bodies. Thus, the scientific community shoulders the responsibility of contributing to the waste treatment by developing effective dye removal technique.
Dyes can have acute and/or chronic effects on exposed organisms depending on the exposure time and dye concentration. Dyes can cause allergic dermatitis, skin irritation, cancer, mutation, etc. Dyes can be classified as (Mishra and Tripathy 1993): anionic (direct, acid and reactive dyes), cationic (basic dyes) and non-ionic (dispersive dyes).
Many treatment processes have been applied for the removal of dye from wastewater such as: Fenton process (Behnajady et al. 2007), photo/ferrioxalate system (Huang et al. 2007), photo-catalytic and electrochemical combined treatments (Neelavannan et al. 2007), photo-catalytic degradation using UV/TiO2 (Sohrabi and Ghavami 2008), sono-chemical degradation (Abbasi and Asi 2008), Fenton-biological treatment scheme (Lodha and Chaudhari 2008), biodegradation (Daneshvar et al. 2007), photo-Fenton processes (Garcia-Montano et al. 2007), integrated chemical–biological degradation (Sundarjanto et al. 2006), electrochemical degradation (Fan et al. 2008), adsorption process (Tan et al. 2007; Hameed et al. 2007a, b), chemical coagulation/flocculation, ozonation, cloud point extraction, oxidation, nano-filtration, chemical precipitation, ion-exchange, reverse osmosis and ultra-filtration (Lorenc-Grabowsk and Gryglewic 2007; Malik and Saha 2003; Malik and Sanyal 2004; Banat et al. 1996).
Among treatment technologies, adsorption is rapidly gaining prominence as a method of treating aqueous effluent. Some of the advantages of adsorption process are possible regeneration at low cost, availability of known process equipment, sludge-free operation and recovery of the sorbate (Kapdan and Kargi 2002). Activated carbon is the most widely used adsorbent for dye removal because of its extended surface area, micro-pore structures, high adsorption capacity and high degree of surface reactivity. However, commercially available activated carbon is very expensive and has high regeneration cost while being exhausted. Furthermore, generation using solution produces a small additional effluent while regeneration by refractory technique results in a 10–15 % loss of adsorbent and its uptake capacity (Waranusantigul et al. 2003). This has lead to search for cheaper substances. Researchers are always in a hunt for developing more suitable, efficient and cheap and easily available types of adsorbents, particularly from the waste materials.
Reported adsorption capacities qm (mg/g) of different agricultural wastes
Maximum adsorption capacity (mg/g)
Namasivayam and Kavitha (2002)
Rajeswari et al. (2001)
Basic blue 9
Annadurai et al. (2002)
Acid yellow 36
Basic blue 9
Kannan and Sundaram (2001)
Basic blue 9
Banat et al. (2003a)
Oil palm fiber: activated carbon
Hameed and El-Khaiary (2008a)
Durian shell: based activated carbon
Hameed and Hakimi (2008)
Guava (Psidium guajava) leaf Powder
Ponnusami et al. (2008)
Direct red 80
Ardejani et al. (2008)
Pomelo (Citrus grandis peel)
Hameed et al. (2008a)
Broad bean peel
Hameed and El-Khaiary (2008b)
Citrullus lanatus rind
Bharathi and Ramesh (2012)
Removal of dyes by low-cost sorbents
Garlic peel was investigated by Hameed and Ahmad (2009) for the removal of Methylene blue from aqueous solution. Equilibrium isotherms were determined and analyzed using the Langmuir, Freundlich and Temkin isotherms. The maximum monolayer adsorption capacities were found to be 82.64, 123.45 and 142.86 mg g−1 at 303, 313 and 323 K, respectively. Batch studies were carried out to explore the potential use of garlic peel as low-cost adsorbent for Methylene blue removal from aqueous solution. The kinetic data were analyzed using pseudo-first-order and pseudo-second-order models. For Methylene blue author observed that the adsorption capacity was higher due to the presence of polar functional group. Dogan et al. (2009) studied hazelnut shell, an agricultural waste, without any pretreatment for the removal of Methylene blue. Pine apple stem was studied by Hameed et al. (2009) for the adsorption of Methylene blue (basic dye) from aqueous solution. The process was studied at different concentration of dyes, contact time, and pH and was found to obey the Langmuir isotherm. The authors suggested that the acidic pH is favorable for the adsorption. The maximum adsorption capacity on pine apple stem for the removal of Methylene blue was found to be 119.05 mg g−1.
Jack fruit peel has been investigated as adsorbents for removal of Methylene blue by Hameed (2008a). The effect of different system variables like adsorbent dose, initial dye concentration, contact time and pH were evaluated and found that as the amount of adsorbent increased, the percentage of dye removal increased accordingly. Low concentrations of Methylene blue favored high adsorption percentages and the optimum pH value for dye adsorption was found to be 4.0. The equilibrium biosorption data were analyzed using four different types of linearized Langmuir isotherm, the Freundlich isotherm and the Temkin isotherm. Best fits were obtained with the type 2 Langmuir model. The sorption capacity of Methylene blue on jack fruit peel was found to be 285.713 mg g−1.
Oil palm trunk fiber as an adsorbent was investigated by Hameed and El-Khaiary (2008a) who studied the removal of Malachite green, thereby making an attempt to overcome the economic disadvantages of activated carbon. The adsorbent was studied without any pretreatment and was sieved into different size ranges prior to use. The monolayer coverage of Malachite green on oil palm trunk fiber was found to be 149.35 mg g−1 at 30 °C.
Wang et al. (2008) reported on the capacity and mechanism of adsorption of two basic dyes, namely Malachite green and Methylene blue by rice bran and wheat bran. Rice bran and wheat bran are by-products. The adsorption of both basic dyes was pH dependent. Both the dyes are basic in nature, which upon dissociation release colored dye cations into solution. The adsorption of these positively charged dye groups on to the adsorbent is primarily influenced by the surface charge on the adsorbent, which in turn is influenced by the surface charge on the adsorbent, which in turn is influenced by the solution pH. As the pH is increased, greater cation removal is facilitated. The kinetic experimental data were analyzed using four kinetic equations including pseudo-first-order equation, pseudo-second-order equation, external diffusion model and intra-particular diffusion model. The experimental data were fitted with Langmuir and Freundlich isotherms and the results showed that the Langmuir isotherm exhibited a little better fit to the Methylene blue adsorption data by both adsorbents. While, the Freundlich isotherm seemed to agree better with the Malachite green adsorption, the effects of particle size, adsorbent concentration and solution ionic strength on the adsorption of the two dyes were studied and it was found that the adsorption capacity decreases with an increase in the adsorbent concentration. This is due to the fact that some of the adsorption sites remained unsaturated during the adsorption process and due to inter-particular interaction.
Broad bean peel an agricultural waste chopped, sieved, washed and oven dried at 60 °C for 48 h was used by Hameed and El-Khaiary (2008b) for removal of cationic dye (Methylene blue) and adsorption capacity of 192.7 mg g−1 was found. It was noted that adsorption of dye decreases with an increase in the initial Methylene blue concentration. The adsorption of dyes was reported to follow Langmuir adsorption model and pseudo-first-order kinetic model.
Groundnut shell, an agricultural solid waste has been used as an adsorbent by Malik et al. (2007), for the removal of Malachite green from aqueous solution. The material is largely available and can be used as a potential sorbents due to their physico-chemical characteristics and low cost. Groundnut shell is easily available at zero prices. Nut shell is carbonaceous, fibrous solid waste, which creates a disposal problem and is generally used for its fuel value. Further, in order to know the effect of chemical treatment and improve its efficiency, the authors also tested the potential of the adsorbents by treating it with ZnCl2. Besides this, the simulation studies for effect of contact time, adsorbent dose and initial dye concentration were also studied. The experimental results indicated that at a dose of 0.5 g L−1 and initial concentration of 100 mg L−1, groundnut shell powder activated carbon showed 94.5 % removal of the dye in 30 min equilibrium time, while commercially available powdered activated carbon removed 96 % of the dye in 15 min. The experimental isotherm data were analyzed using the linearized form of Freundlich, Langmuir and BET equations to determine the maximum adsorptive capacities. The equilibrium data fit well to the Freundlich isotherm.
Raw agricultural solid wastes and waste materials from forest industries such as sawdust have been used as adsorbents. These materials are available in large quantities and may have potential as adsorbents due to their physico-chemical characteristics and low cost. Sawdust is an abundant by-product of the wood industry, which is available in country side at zero or negligible price. It contains various organic compounds (lignin, cellulose and hemicellulose) with poly phenolic groups that might be useful for binding dyes through different mechanisms. The role of sawdust material in the removal of pollutants from aqueous solutions has been reviewed recently by Shukla et al. (2002). Sawdust has proven to be a promising effective material for the removal of dyes from wastewater. Garg et al. (2003) studied Rose wood sawdust a low-cost adsorbent for the removal of Malachite green from aqueous solution. Further, in order to know the effect of chemical treatment and to improve its efficiency the authors also tested the potential of the adsorbent by treating it with formaldehyde and sulphuric acid. Besides this, studies on the effect of pH, initial concentration, adsorbent dose and contact time were also carried out by Garg et al. (2003). The authors determined that an initial pH in the range of 6–9 was favorable for dye removal. The low adsorption of Malachite green at acidic pH was suggested to be due to the presence of H+ ions that compete with the dye cation for adsorption sites. With the increase of the pH of the system, the number of positively charged sites decreases while the number of the negatively charged increases.
Dulman and Cucu-Man (2009) investigated the effect of Beech wood sawdust on the adsorption of six reactive dyes in aqueous solution, namely C.I. Direct Blue 6, C.I. Direct Brown 2, C. I. Direct Green 26, C.I. Direct Brown, C.I. Reactive Red 3. C.I. Basic Blue 86. The percentage removal of the reactive dyes Direct Brown 2 and Direct Brown decreased with increase in pH (above pH 10) and the maximum removal rate was occurred at pH 3. Consequently, the percentage color removal of Direct Brown 2 and Direct Brown dropped from 98.6 to 34.7 % and 94.4 to 28.5 %, respectively. For Basic Blue the sorption has a maximum value of 97 % at pH 4.43–7.06. At lower pH (pH < pHzpc), the percentage color removal of hydrolyzed reactive dyes was relatively high. Malik (2003) investigated Mahogany sawdust and rice husk as adsorbents for the removal of (acidic dye) Acid yellow 36. The adsorbents were activated by means of steam. The kinetics of the process was found to be dependent on contact time, adsorbent dose and pH. The authors found that an acidic pH is favorable for the adsorption of acid dye. It was observed that adsorption obeys both Freundlich and Langmuir isotherms and the intraparticle diffusion of dye molecule within the particle is the rate-limiting step. The monolayer coverage of acid yellow 36 on Mahogany sawdust was found to be 183.3 mg g−1 of the adsorbent. Hameed et al. (2007a) studied rattan sawdust as adsorbent for the removal of Malachite green from aqueous solution. The adsorbent was studied without any physical or chemical treatment. The equilibrium data fit with the Langmuir isotherm with a monolayer capacity of 62.71 mg g−1. The authors found that for a short time period the rate of adsorption is controlled by film diffusion. However, at longer adsorption times, pore diffusion controls the rate of adsorption
Hameed (2009a), studied papaya seeds a novel non-conventional low-cost adsorbent for the removal of (cationic dye) Methylene blue. The effect of dye adsorption increased with increase in adsorbent dosage and pH. In terms of the initial rate of adsorption, the uptake of the cationic dye on to papaya seeds was found to occur more rapidly. The intraparticle diffusion indicated that more than one process affected the adsorption. The removal of Methylene blue by papaya seeds suggested that the sorption interaction obeyed the pseudo-second-order kinetics. The equilibrium data for Methylene blue on papaya seeds were modeled with the Langmuir, Freundlich, and Temkin models. The data fitted well with the Langmuir model with a maximum monolayer capacity of 555.557 mg g−1.
Leaf biomass, an agricultural waste, widely available was studied as an alternative adsorbent for different pollutants as well as dyes by various investigators (Ponnusami et al. 2009; Weng et al. 2009; Han et al. 2007; Immich and Ulson de Souza 2009). The plant leaves have porous structure which can effectively adsorb dye molecules. The functional groups on the leaf surface can attract ionic dye molecules of opposite charge which lead to increase in dye removal efficiency. Ponnusami et al. (2009) studied Gulmohar (Delonix regia) as adsorbent for the removal of Methylene blue from aqueous solution. The materials were studied without chemical treatment. Authors found the adsorption was favorable at higher pH and lower temperature. The equilibrium data were well fitted by the Langmuir isotherm an appreciable Langmuir capacity of 0.3 mg g−1 was found out.
A Phoenix tree leaf has also been studied as an adsorbent by Han et al. (2007), for the removal of Methylene blue from aqueous solution. The Phoenix tree leaves contain abundant floristic fiber, protein and some functional groups such as carboxyl, hydroxyl and amidogen, etc., which make biosorption process possible. The leaf is a waste product with practically no cost but its adsorption capacity is 80.90, 83.80, 89.70 mg g−1 at 295, 305 and 323 K, respectively, makes it an adsorbent of a little importance for dye removal from wastewater. Neem leaf has proven to be a promising effective material for the removal of Remazol Blue RR dye from aqueous solution (Immich and Ulson de Souza 2009). Pine apple leaf powder an agricultural waste, has been recently investigated to remove Methylene blue from aqueous solutions by Weng et al. (2009). Pine apple leaf powder is a complex material containing 70–80 % cellulose, lignin (5–12 %) and hemicellulose. The maximum adsorption capacity varied from 0.15 mg/g only. The capacity increased as the initial Methylene blue concentration increases. The adsorption increases with decreasing temperature suggesting that the adsorption reaction is exothermic in nature.
Namasivayam et al. (2001) investigated coir pith, an agricultural solid waste, as an adsorbent for the adsorption of Rhodamine B and Acid violet dyes. The adsorbent was used after drying, sieving and carbonizing at 700 °C. It was found that Rhodamine B adsorption reached equilibrium stage at 5, 7, 10 and 10 min for dye concentration 10, 20, 30 and 40 mg L−1, respectively, while crystal violet (CV) was found to have equilibrium time of 40 min for all the concentrations. The adsorption capacity was found to be 2.56 and 8.06 mg g−1 of adsorbent for Rhodamine B and Acid violet, respectively. Coir pith has also been investigated as an adsorbent by Kavitha and Namasivayam (2007) for the removal of Procion Orange from wastewater. The sorption capacity of 2.6 mg g−1 makes it an adsorbent of little importance for dye removal from wastewater. Banana stalks were studied as adsorbents by Hameed et al. (2008b) for basic dyes in aqueous solutions with equilibrium isotherms and kinetic adsorptions. High adsorption capacity of 243.90 mg g−1 was observed and authors suggested that banana stalks consists of cellulose and lignin; it is the polyol structure of cellulose-based materials that has relatively strong chemical adsorption of cations such as metal ions and organic bases as well as physical adsorption of other material such as acidic and anionic compounds.
Mall et al. (2006) utilized bagasse fly ash for the removal of Orange-G (OG) and Methyl violet (MV) from aqueous solution. Results indicated that OG is strongly adsorbed at pH 4.0, whereas MV is strongly adsorbed at pH 9.0. The percentage of dye removal was higher at low initial concentration and increased in amount of adsorbent used. The adsorption data have been correlated with Freundlich, Langmuir, Redlich–Peterson, Dubinin–Radushkevich and Tempkin adsorption models. The authors observed that the Freundlich isotherm gave the best correlation for the adsorption of Orange-Green-bagasse fly ash system and Redlich–Peterson isotherm better fits the Methyl violet-bagasse fly ash system. The adsorption of Methylene violet and Orange Green followed pseudo-second-order kinetics. Manaskorn et al. (2004), studied bagasse pith from sugarcane industry without any pretreatment for the removal of three reactive dyes, Remazol Black B, Remazol Brilliant Blue and Remazol Brilliant Red from aqueous solutions. High percentage removal was observed for the adsorption of reactive dyes in the order of 58.48–98.03 % for RR Black, 46.15–93.47 % for RB Blue and 46.30–94.60 % for RB Red, respectively.
Agricultural solid waste such as seed hull has been used as adsorbents for the removal of dye from wastewater. These materials are available in large quantities and may have potential as adsorbents due to their physico–chemical characteristics and low cost. Sunflower seed hull activated with sulphuric acid has been used for the removal of Acid violet 17 by Thinakaran et al. (2008). The Langmuir adsorption capacity was found to be 116.27 mg g−1. The same material has been used for the removal of Methyl violet by Hameed (2008b), without any physical or chemical treatment. The equilibrium data were analyzed using the Langmuir, Freundlich and Temkin isotherm models and the equilibrium process was described well by the Freundlich isotherm model. The maximum sorption capacity was found to be 92.59 mg L−1 at 30 °C. Pumpkin seed hull as low-cost adsorbent has been investigated by Hameed and El-Khaiary (2008a), for the removal of basic dye (Methylene blue) from aqueous solutions. Authors noted that adsorption of dyes was rapid on the outer surface, followed by slower adsorption inside the porous. The removal of Methylene blue was high at pH 6–9. The results obtained by the workers indicated that the multilayer adsorption isotherm was found to have the best fit to the experimental data, suggesting multilayer adsorption on a homogeneous surface. The adsorption capacity was determined from the parameters of adsorption isotherms and was found to be 141.92 mg g−1.
Hevea brasiliensis seed coat was studied by Hameed and Daud (2008), for the adsorption of basic blue from aqueous solutions with different contact time and initial concentration. The monolayer adsorption capacity was found to be 227.27 mg g−1 at 30 °C. Authors reported that adsorption process obeyed the pseudo-second-order kinetic model and the adsorption isotherm followed Freundlich isotherm model. Thinakaran et al. (2008) investigated gingelly (sesame) (sp), cotton (cp), pongam (pp) seed hulls, an agricultural waste for the adsorption of Acid Red 114 from aqueous solution. The materials were used after cleaning, drying, soaking in 18 N H2SO4 and carbonizing at 80 °C. It was found that the optimum condition for AR114 removal was at a pH of 3, adsorbent dose of 3 g L−1 and at an equilibrium time of 4 h. The adsorption capacity was in the order of sp > cp > pp. Another agricultural product is bamboo, a grass, the most diverse group of plants in the grass family. Bamboo is an abundant natural resource which has been found to be effective in retaining dyes from aqueous solutions. Because of its low cost and high availability, bamboo is very attractive as an adsorbent. Like sawdust, the cost of forest waste is only associated with the transport cost from the storage place to the site where they will be utilized. The adsorption of Methylene blue on to bamboo-based activated carbon was studied by Hameed et al. (2007b). In order to improve the efficiency, the authors also tested the potential of the adsorbent by treating it with potassium hydroxide and CO2. Besides this, the simulation studies for the effect of agitation time and concentration of dye were also carried out. The equilibrium data for Methylene blue adsorption well fitted to the Langmuir equation, with maximum monolayer adsorption capacity of 454.2 mg g−1. Hameed (2009b), studied grass an agricultural waste without any pretreatment for the removal of basic dyes (Methylene blue) from aqueous solution. The agricultural waste was found to have high adsorption capacity of 457.60 mg g−1. Other agricultural solid wastes from cheap and readily available resources such as de-oiled soya (Mittal et al. 2005) date pits (Banat et al. 2003b), coir pith, sawdust, sugarcane fiber (Parab et al. 2009), banana pith (Kadirvelu et al. 2003; Ho and McKay 1999; Chen et al. 2001), corncob (Robinson et al. 2002b, c) and orange peel (Namasivayam et al. 1996) have also been successfully employed for the removal of dyes from aqueous solutions.
Adsorption kinetics depends on the adsorbate–adsorbent interaction and system condition and has been investigated for their suitability for application in water pollution control. Two vital evaluation elements for an adsorption process operation unit are the mechanism and the reaction rate. Solute uptake rate determines the residence time required for completing the adsorption reaction and can be enumerated from kinetic analysis. Numerous attempts were made in formulating a general expression to describe the kinetics of adsorption on solid surfaces for the liquid–solid adsorption system (Ho 2004). The adsorption rate is an important factor for a better choice of material to be used as an adsorbent; where the adsorbent should have a large adsorption capacity and a fast adsorption rate. Most of adsorption studies used pseudo-first-order and pseudo-second-order models to study the adsorption kinetics (Salleh et al. 2011).
If the adsorption fits the Elovich model, a plot of q t versus ln (t) should yield a linear relationship with a slope of (1/β) and an intercept of (1/β) ln (αβ).
The value of RL indicates the type of the isotherm to be either unfavorable (RL > 1), linear (RL = 1), favorable (0 < RL < 1) or irreversible (RL = 0).
T is the absolute temperature in Kelvin and R is the universal gas constant, 8.314 J mol−1 K−1. The constant B T is related to the heat of adsorption, A T is the equilibrium binding constant (L g−1) corresponding to the maximum binding energy. The slope and intercept from a plot of q e versus ln C e determines the isotherm constants A T and B T .
The adsorption capacity for cationic dye adsorption is higher than anionic dye adsorption on the same adsorbent (Salleh et al. 2011). Since the carboxyl group is one of the major functional groups in agricultural wastes, it will have an effect on the adsorption capacity according to the dye class. The carboxyl group bears a negative charge, and therefore it is the major functional group in the adsorption of cationic dyes. On other hand, it will inhibit the adsorption of anionic dyes (Gong et al. 2005).
Factors affecting adsorption
Effect of initial dye concentration
Effect of adsorbent dosage
Effect of contact time
The effect of contact time on adsorption of dye can be carried out by preparing adsorbent–adsorbate solution with fixed adsorbent dose and initial dye concentration for different time intervals and shaken until equilibrium. Generally the rate of removal of dye increases with an increase in contact time to a certain extent. Further increase in contact time does not increase the uptake due to deposition of dyes on the available adsorption site on adsorbent material (Ansari and Mosayebzadeh 2010). At this point, the amount of the dye desorbing from the adsorbent is in a state of dynamic equilibrium with the amount of the dye being adsorbed onto the adsorbent. The time required to attain this state of equilibrium is termed the equilibrium time, and the amount of dye adsorbed at the equilibrium time reflects the maximum adsorption capacity of the adsorbent under those operating conditions (Bello et al. 2010).
Effect of pH
Effect of agitation speed
Effect of ionic strength
The wastewater containing dye has commonly higher salt concentration, and effects of ionic strength are of some importance in the study of dye adsorption onto adsorbents (Han et al. 2007). The effect of ionic strength on adsorption can be carried out by adding different doses of salts (normally NaCl) to the adsorbent–adsorbate solution and shaking up to equilibrium time. Theoretically, when the electrostatic forces between the adsorbent surface and adsorbate ions were attractive, as in this system, an increase in ionic strength will decrease the adsorption capacity. Conversely, when the electrostatic attraction is repulsive, an increase in ionic strength will increase adsorption (Newcombe and Drikas 1997; Alberghina et al. 2000; Germa’n-Heins and Flury 2000). Wang et al. (2008) reported that the extent of adsorption is sensitive to changes in concentration of supporting electrolyte (chloride sodium) indicates that electrostatic attraction may be a significant component of the overall adsorption in this system. The electrostatic free energy change, ∆G contributes to the total free energy change of adsorption, ∆G and depends on the ionic strength of solution. When the ionic strength was increased, the electrical double layer surrounding the adsorbent surface was compressed, which would lead to a decrease in the electrostatic potential. This indirectly resulted in a reduction in the coulombic free energy, and a decrease in basic dye ions adsorption. Arivoli et al. (2009) reported that the low concentration NaCl solution had little influence on the adsorption capacity. When the concentration of NaCl increases, the ionic strength is raised. At higher ionic strength, the adsorption of Malachite green will be higher owing to the partial neutralization of the positive charge on the carbon surface and a consequent compression of the electrical double layer by the Cl− anion. The chloride ion also enhances adsorption of Malachite green ion by pairing their charges, and hence reducing the repulsion between the Malachite green molecules adsorbed on the surface. This initiates carbon to adsorb more positive Malachite green ions (Arivoli 2007; Guo et al. 2005). Wang et al. (2008) examined three competitive modes (competitive mode, uncompetitive mode and noncompetitive mode) to quantify the ionic strength effects. According to the competitive mode, the sodium ions interact directly with the active sites on the adsorbent surface, competing with basic dye for the available sites. For the competitive isotherm, the intercept term of the linearized Langmuir isotherms remains constant. For uncompetitive inhibition, the sodium ions do not react with the active sites on the adsorbent surface directly, but instead react with the adsorbent surface–dye complexes. In this case, the linearized Langmuir adsorption isotherms remain parallel to each other. Noncompetitive mode mechanism is a combination of the above two modes. Both the sodium ions and basic dye adsorb independently at different sites on the adsorbent surface. In other words, sodium ions react with the adsorbent surface sites and dye molecules adsorbent surface complexes, while dye molecules react with the adsorbent surface active sites and sodium ions–adsorbent surface complexes. In this case, the linearized Langmuir isotherms converge at x axis.
Effect of temperature
A study of the temperature dependence of adsorption reactions gives valuable knowledge about the enthalpy and entropy changes during adsorption (Alkan and Doğan 2003). Temperature is an indicator for the adsorption nature whether it is an exothermic or endothermic process (Salleh et al. 2011). If the adsorption capacity increases with increasing temperature then the adsorption is an endothermic process. This may be due to increasing the mobility of the dye molecules and an increase in the number of active sites for the adsorption with increasing temperature (Senthilkumaar et al. 2006). Senthilkumaar et al. (2006) reported that the enhancement of adsorption capacity of the activated carbon at higher temperatures is attributed to the enlargement of pore size and activation of the adsorbent surface. During the adsorption there, some structural changes in the dyes and the adsorbent occur (Hema and Arivoli 2007). The adsorbed water molecules, which are displaced by the adsorbate species, gain more translational entropy than it is lost by the adsorbate molecules, thus allowing the prevalence of randomness in the system. Increasing temperature may decrease the adsorptive forces between the dye species and the active sites on the adsorbent surface as a result of decreasing adsorption capacity (Ofomaja and Ho 2007).
Mechanism of adsorption
Transport of the adsorbate ions to the external surface of the adsorbent (film diffusion).
Transport of the adsorbate particles within the pores of adsorbent, excluding the small amount of adsorption occurring at the external surface of the adsorbent (particle diffusion).
Adsorption of the adsorbate ions on the interior surface of the adsorbent.
If external transport < internal transport, particle diffusion will take place and while external transport > internal transport, adsorption is governed by film diffusion process. If external transport ≈ internal transport, the transport of the adsorbate ions to the boundary may not be possible with a significant rate because of which there is a possibility of formation of a liquid film around the solid adsorbent particles (Gupta et al. 2004).
Modifications of adsorbents
In order to increase the adsorption capacity of the adsorbent, researchers have followed different activation methods and they usually used the Langmuir isotherm to indicate the effectiveness of the activation process. Activation methods involve physical activation such as carbonization of material and chemical activation such as using chemical activating agents (Salleh et al. 2011). Abdelwahab et al. (2005) treated rice husk with citric acid for treating synthetic Direct F. Scarlet (Direct Red 23) containing industrial wastewater. The authors reported that the activated rice husk possesses the highest sorption capacity, especially for 2.5 and 5 g L−1 of sorbent. The removal curves are single, smooth and continuous leading to saturation. Activated rice husk is observed to have higher adsorption capacity than the untreated rice husk in the removal of Direct Red-23. Formaldehyde-treated sawdust was used by Bello et al. (2010) for removing Methylene blue from aqueous solution. Garg et al. (2004) treated Prosopis cineraria tree saw dust with formaldehyde and sulphuric acid for removing Malachite green. The authors reported that the optimum pH for dye removal by formaldehyde-treated Prosopis cineraria sawdust and sulphuric acid-treated Prosopis cineraria sawdust was 6–10. Higher dye removal by sulphuric acid-treated Prosopis cineraria sawdust and formaldehyde-treated Prosopis cineraria sawdust was possible provided the initial dye concentration was low in solution. The adsorption capacity of formaldehyde-treated Prosopis cineraria sawdust is less than that of sulphuric acid-treated P. cineraria sawdust. Low and Lee (1990) treated coconut husk with a mixture of formaldehyde/HCl for removing Methylene blue from aqueous solution. Sharma and Uma (2010) prepared activated carbon by pyrolyzing rice husk, in the presence of ZnCl2. They reported that the activated carbon displayed both microporous and mesoporous nature with a significant surface area of 180.50 m2 g−1. Water hyacinth roots were treated with 2 N HCl by Rajamohan (2009) for removing Congo red. Kumar and Ahmad (2011) TGW with H2SO4 and ZnCl2 for removing crystal violet from aqueous solution. Wood sawdust obtained from walnut and its polypyrrole coated form for the removal of Methylene blue from aqueous solutions was used by Ansari and Mosayebzadeh (2010). They reported that sawdust and its polypyrrole coated form have maximum monolayer adsorption capacity of 19.41 and 34.36 mg g−1, respectively. Hema and Arivoli (2007) used carbonized leaves of Pandanus with concentrated sulphuric acid in the weight ratio of 1:1 (W/V) for removing Congo red, Malachite green and Rhodamine B.
Ferric chloride orthophosphoric acid treated > potassium carbonate treated > raw coir pith.
Ferric chloride orthophosphoric acid treated > potassium carbonate treated = trioxonitrate acid treated > raw
Ferric chloride orthophosphoric acid treated > raw > trioxonitrate acid treated > potassium carbonate treated
Desorption studies help to elucidate the nature of adsorption and recycling of the spent adsorbent and the dye. If the adsorbed dyes can be desorbed using neutral pH water, then the attachment of the dye by the adsorbent will be weak bonds. If sulphuric acid or alkaline water desorbs the dye then the adsorption will be through ion-exchange. If an organic acid, such as acetic acid can desorbs the dye, then the dye has been held by the adsorbent through chemisorption (Arivoli et al. 2009). Desorption process usually done by mixing a suitable solvent with the dye-saturated substrate and shaken together for fixed time, until the dye extract on the solvent and then using filtration to separate the adsorbent. The dye–solvent mixture dried at high temperature to evaporate the solvent. The desorbed dye then determine in spectrophotometer (Robinson et al. 2002a). Mahmoodi et al. (2011) studied the desorption of three textile dyes from pinecone and they concluded that the maximum desorption for Acid black 26, Acid green 25 and Acid blue 7 was 93.16, 26.97 and 98 %, respectively. Bello et al. (2010) reported that effect of various reagents used for desorption studies shows that hydrochloric acid is a better reagent for desorption, because we could get more than 90 % removal of adsorbed dyes. Also, the adsorbent exhibits a stable structure towards this reagent. The desorption of dyes by mineral acids indicates that the dyes are adsorbed onto treated sawdust by physisorption. Similar results were reported by Arivoli et al. (2009). Somasekhara Reddy (2006) reported that percent desorption of Congo red dye from tamarind fruit shell increases with increase in pH of solution. Robinson et al. (2002a) studied desorption of Cibacron red from corncob using mixture of methanol, chloroform and water. They found that the maximum value of desorption was 93 %. Kumar and Ahmad (2011) studied the desorption of crystal violet dye from ginger waste and they found that NaOH and H2O did not showed any desorption while acetic acid desorbed about 35–50 % of dye. Ansari and Mosayebzadeh (2010) used different chemicals for the recovery of Methylene blue.
In this review, a wide range of agricultural waste materials, as low-cost adsorbent has been presented. The use of these low-cost biosorbents is recommended since they are relatively cheap or of no cost, easily available, renewable and show highly affinity for dyes. The process of biosorption requires further investigation in the direction of modeling, regeneration of biosorbent and immobilization of the waste material for enhanced efficiency and recovery. Further more interest should be concentrated by the researchers to predict the performance of the adsorption process for dye removal from real industrial effluents.
- Abbasi M, Asi NR (2008) Sonochemical degradation of Basic Blue 41 dye assisted by nano TiO2 and H2O2. J Hazard Mater 153:942–947Google Scholar
- Abdelwahab O, Nemr AE, Sikaily AE, Khaled A (2005) Use of rice husk for adsorption of direct dyes from aqueous solution: a case study of Direct f. Scarlet. Egypt J Aquat Res 31:1–11Google Scholar
- Adekola FA, Adegoke HI (2005) Adsorption of blue-dye on activated carbons produced from rice husk, coconut shell and coconut coir pith. J Sci 7:151–157Google Scholar
- Aksu Z, Tezer S (2005) Biosorption of reactive dyes on the green alga Chlorella vulgaris. J Process Biochem 40:1347–1361Google Scholar
- Alberghina G, Bianchini R, Fichera M, Fisichella S (2000) Dimerization of Cibacron Blue F3GA and other dyes: influence of salts and temperature. Dyes Pigment 46:129–137Google Scholar
- Alkan M, Doğan M (2003) Adsorption kinetics of Victoria blue onto perlite. Fresenius Environ Bull 125:418–425Google Scholar
- Allen SJ, Koumanova B (2003) Decolourisation of water/wastewater using adsorption. J Univ Chem Technol Metall 40:175–192Google Scholar
- Annadurai G, Juang RS, Lee DJ (2002) Use of cellulose-based wastes for adsorption of dyes from aqueous solutions. J Hazard Mater B92:263–274Google Scholar
- Ansari R, Mosayebzadeh Z (2010) Removal of basic dye methylene blue from aqueous solutions using sawdust and sawdust coated with polypyrrole. J Iran Chem Soc 7:339–350Google Scholar
- Ardejani FD, Badii K, Nimall NY, Shafaei SZ, Mirhabibi AR (2008) Adsorption of direct red 80 dyes from aqueous solution on to almond shells: effect of pH, initial concentration and shell type. J Hazard Mater 151:730–737Google Scholar
- Arivoli S (2007) Kinetic and thermodynamic studies on the adsorption of some metal ions and dyes onto low cost activated carbons. Ph D. Thesis, Gandhigram Rural University, GandhigramGoogle Scholar
- Arivoli S, Hema M, Prasath PMD (2009) Adsorption of Malachite green onto carbon prepared from Borassus bark. Arab J Sci Eng 34:31–42Google Scholar
- Banat IM, Nigam P, Singh D, Marchant R (1996) Microbial decolorization of textile-dye-effluents: a review. Bioresour Technol 58:217–227Google Scholar
- Banat F, Al-Asheh S, Al-Makhadmeh L (2003a) Evaluation of the use of raw activated date pits as potential adsorbents for dye containing waters. J Chem Technol Biotech 54:192–196Google Scholar
- Banat F, Al-Asheh S, Al-Makhadmeh L (2003b) Evaluation of the use of raw and activated date pits as potential adsorbents for dye containing waters. Process Bio Chem 39:193–202Google Scholar
- Behnajady MA, Modirshahla N, Ghanbary F (2007) A kinetic model for the decolorization of C. I. Acid yellow 23 by Fenton process. J Hazard Mater 148:98–102Google Scholar
- Bello OS, Adelaide OM, Hammed MA, Popoola OAM (2010) Kinetic and equilibrium studies of methylene blue removal from aqueous solution by adsorption on treated sawdust. Macedonian J Chem Eng 29:77–85Google Scholar
- Benaïssa H (2005) Removal of acid dyes from aqueous solutions using orange peel as a sorbent material. Ninth International Water Technology Conference, IWTC9, Sharm El-Sheikh, Egypt, pp 1175–1185Google Scholar
- Bharathi KS, Ramesh ST (2012) Equilibrium, thermodynamic and kinetic studies on adsorption of a basic dye by Citrullus lanatus rind. Iran J Energy Environ 3(1):23–34Google Scholar
- Bhattacharya AK, Venkobachar C (1984) Removal of cadmium II by low cost adsorbents. J Environ Eng Am Soc Civil Eng 110:110–122Google Scholar
- Boyd GE, Adamson AW, Mayers LS (1947) The exchange adsorption of ions from aqueous solution by organic zeolites. II. Kinetics. J Am Chem Soc 69:2836–2848Google Scholar
- Bulut Y, Aydin H (2006) A kinetics and thermodynamics study of Methylene blue adsorption on wheat shells. Desalination 194:259–267Google Scholar
- Chen B, Hui CW, McKay G (2001) Film-pore diffusion modeling and contact time optimization for the adsorption of dye stuffs on pith. Chem Eng J 84:77–94Google Scholar
- Chien SH, Clayton WR (1980) Application of Elovich equation to the kinetics of phosphate release and sorption on soils. Soil Sci Soc Am J 44:265–268Google Scholar
- Crini G, Peindy HN, Gimber F, Robert C (2007) Removal of C.I. basic green 4 Malachite green from aqueous solutions by adsorption using cyclodextrin-based adsorbent: kinetic and equilibrium studies. Sep Purif Technol 53:97–110Google Scholar
- Dalal RC (1974) Desorption of phosphate by anion exchange resin. Commun Soil Sci Plant Anal 5:531–538Google Scholar
- Daneshvar N, Khatae AR, Rasoulifard MH, Pourhassan M (2007) Biodegradation of dye solution containing Malachite green: optimization of effective parameters using Taguchi method. J Hazard Mater 143:214–219Google Scholar
- Dogan M, Abak H, Alkan M (2009) Adsorption of Methylene blue onto Hazelnut shell: kinetics, mechanism and activation parameters. J Hazard Mater 164:172–181Google Scholar
- Dulman V, Cucu-Man SM (2009) Sorption of some textile dyes by beech wood sawdust. J Hazard Mater 162:1457–1464Google Scholar
- Fan L, Zhou Y, Yang W, Chen G, Yang F (2008) Electrochemical degradation of aqueous solution of Amarnath azo dye on ACF under potentiostatic model. Dyes Pigment 76:440–446Google Scholar
- Freundlich H (1906) Über die adsorption in lösungen (Adsorption in solution). J Chem Phys 57:384–470Google Scholar
- Fytianos K, Voudrias E, Kokkalis E (2000) Sorption–desorption behavior of 2,4-dichlorophenol by marine sediments. Chemosphere 40:3–6Google Scholar
- Garcia-Montano J, Ruiz N, Munoz I, Domenech X, Garcia-Hortal JA, Tor-rades F, Pearl J (2007) Environmental assessment of different Photo-Fenton approaches for commercial reactive dye removal. J Hazard Mater 138:218–225Google Scholar
- Garg VK, Gupta R, Yadav RB, Kumar R (2003) Dye removal from aqueous solutions by adsorption on treated sawdust. Bioresour Technol 89:121–124Google Scholar
- Garg VK, Rakesh K, Renuka G (2004) Removal of Malachite green dye from aqueous solution by adsorption using agro-industry waste: a case study of Prosopis cineraria. Dyes Pigment 62:1–10Google Scholar
- Geopaul N (1980) Some methods for the utilization of waste from fiber crops and fiber waste from other crops. Agric Waste Manage 2(3):13–18Google Scholar
- Germa’n-Heins J, Flury M (2000) Sorption of Brilliant Blue FCF in soils as affected by pH and ionic strength. Geoderma 97:87–101Google Scholar
- Gong R, Ding Y, Li M, Yang C, Liu H, Sun Y (2005) Utilization of powdered peanut hull as biosorbent for removal of anionic dyes from aqueous solution. Dyes Pigment 64:187–192Google Scholar
- Goswami S, Ghosh UC (2005) Studies on adsorption behaviour of Cr(VI) onto synthetic hydrous stannic oxide. Water SA 31(44):57–602Google Scholar
- Guo Y, Zhao J, Zhang H, Yang S, Wang Z, Xu H (2005) Use of Rice husk based porous carbon for the adsorption Rhodamine B from aqueous solution. Dyes Pigment 66:123–128Google Scholar
- Gupta VK, Mittal A, Krishnan L, Gajbe V (2004) Adsorption kinetics and column operations for the removal and recovery of Malachite green from wastewater using bottom ash. Sep Purif Technol 40:87–96Google Scholar
- Haghseresht F, Lu G (1998) Adsorption characteristics of phenolic compounds onto coal-reject-derived adsorbents. Energy Fuels 12:1100–1107Google Scholar
- Halsey G (1948) Physical adsorption on non-uniform surfaces. J Chem Phys 16:931–937Google Scholar
- Hameed BH (2008a) Removal of cationic dye from aqueous solution using Jack fruit peel as non-conventional low cost adsorbents. J Hazard Mater 39:338–343Google Scholar
- Hameed BH (2008b) Equilibrium and kinetic studies of Methyl violet sorption by agricultural waste. J Hazard Mater 151:316–322Google Scholar
- Hameed BH (2009a) Evaluation of papaya seeds as a novel non-conventional low-cost adsorbent for removal of Methylene blue. J Hazard Mater 162:939–944Google Scholar
- Hameed BH (2009b) A novel adsorbent for the removal of basic dye from aqueous solution. J Hazard Mater 166:233–238Google Scholar
- Hameed BH, Ahmad AA (2009) Batch adsorption of Methylene blue from aqueous solution by garlic peel, an agricultural waste biomass. J Hazard Mater 164:870–875Google Scholar
- Hameed BH, Daud FBM (2008) Adsorption studies of basic dye on activated carbon derived from agricultural waste: Hevea brasiliensis seed coat. Chem Eng J 139:48–55Google Scholar
- Hameed BH, El-Khaiary MI (2008a) Removal of basic dye from aqueous medium using a novel agricultural waste material: pumpkin seed hull. J Hazard Mater 155:601–609Google Scholar
- Hameed BH, El-Khaiary MI (2008b) Sorption kinetics and isotherm studies of a cationic dye using agricultural waste: broad bean peels. J Hazard Mater 154:639–648Google Scholar
- Hameed BH, Hakimi H (2008) Utilization of Durian Durio Zibethinus Murray peel as low cost adsorbent for the removal of Methylene blue from aqueous solution. Biochem Eng J 39:338–343Google Scholar
- Hameed BH, Ahmad AL, Latiff KNA (2007a) Adsorption of basic dye Methylene blue onto activated carbon prepared from rattan sawdust. Dyes Pigment 75:143–149Google Scholar
- Hameed BH, Din ATM, Ahmad AL (2007b) Adsorption of Methylene blue onto bamboo-based activated carbon: kinetics and equilibrium studies. J Hazard Mater 141:819–825Google Scholar
- Hameed BH, Mahmood DK, Ahmad AL (2008a) Sorption of basic dye from aqueous solution by Pomelo citrus grandis peel in a batch system. Colloids Surf A Physicochem Eng Aspects 316:78–84Google Scholar
- Hameed BH, Mahmood DK, Ahmad AL (2008b) Sorption equilibrium and kinetics of basic dye from aqueous solution using banana stalk waste. J Hazard Mater 158:499–506Google Scholar
- Hameed BH, Krishni RR, Sata SA (2009) A novel agricultural waste adsorbent for the removal of cationic dye from aqueous solutions. J Hazard Mater 162:305–311Google Scholar
- Han R, Zou W, Yu W, Cheng S, Wang Y, Shi J (2007) Biosorption of methylene blue from aqueous solution by fallen Phoenix tree’s leaves. J Hazard Mater 141:156–162Google Scholar
- Harkins WD, Jura EJ (1944) The decrease of free surface energy as a basis for the development of equations for adsorption isotherms; and the existence of two condensed phases in films on solids. J Chem Phys 12:112–113Google Scholar
- Hema M, Arivoli S (2007) Comparative study on the adsorption kinetics and thermodynamics of dyes onto acid activated low cost carbon. Int J Phys Sci 2:10–17Google Scholar
- Ho YS (2004) Citation review of Lagergren kinetic rate equation on adsorption reactions. Scientometrics 59:171–177Google Scholar
- Ho YS, McKay G (1998) A comparison of chemisorptions kinetic models applied to pollutant removal on various sorbents. Process Safety Environ Prot 76:332–340Google Scholar
- Ho YS, McKay G (1999) Pseudo-second-order model for sorption processes. Process Bio Chem 34:451–465Google Scholar
- Huang YH, Tsai ST, Huan YF, Chen CY (2007) Degradation of commercial azo dyes reactive Black in photo/ferrioxalate system. J Hazard Mater 140:382–388Google Scholar
- Immich APS, Ulson de Souza AA (2009) Removal of Remazol Blue dye from aqueous solutions with Neem leaves and evaluation of their toxicity with Daphnia magna. J Hazard Mater 164:1580–1585Google Scholar
- Jain AK, Gupta VK, Bhatnagar A, Jain S, Suhas S (2003) A comparative assessment of adsorbents prepared from industrial wastes for the removal of cationic dye. J Indian Chem Soc 80:267–270Google Scholar
- Kadirvelu K, Kavipriya M, Karthika C, Radhika M, Vennilamani N, Pattabhi S (2003) Utilization of various agricultural wastes for activated carbon preparation and application for the removal of dyes and metal ions from aqueous solutions. Bioresour Technol 87:129–132Google Scholar
- Kannan N, Sundaram MM (2001) Kinetics and mechanism of removal of methylene blue by adsorption on various carbons—a comparative study. Dyes Pigment 51:25–40Google Scholar
- Kannan N, Vanangamudi A (1991) A study on removal of chromium VI by adsorption on lignite coal. Indian J Environ Protect 114:241–245Google Scholar
- Kapdan IK, Kargi F (2002) Simultaneous bio degradation and adsorption of textile dye stuff in an activated sludge unit. Process Bio Chem 37:973–981Google Scholar
- Kavitha D, Namasivayam C (2007) Recycling coir pith, an agricultural solid waste, for the removal of Procion orange from wastewater. Dyes Pigment 75:143–149Google Scholar
- Kumar R, Ahmad R (2011) Biosorption of hazardous crystal violet dye from aqueous solution onto treated ginger waste TGW. Desal 265:112–118Google Scholar
- Lagergren S (1898) About the theory of so-called adsorption of soluble substances. Kungliga Svenska Vetenskapsakademiens. Handlingar 244:1–39Google Scholar
- Langmuir I (1915) Chemical reactions at low pressures. J Am Chem Soc 27:1139–1143Google Scholar
- Lodha B, Chaudhari S (2008) Optimization of Fenton biological treatment scheme for the treatment of aqueous dye solution. J Hazard Mater 148:459–466Google Scholar
- Lorenc-Grabowsk E, Gryglewic G (2007) Adsorption characteristics of Congo red on coal-based mesoporous activated carbon. Dyes Pigment 74:34–40Google Scholar
- Low KS, Lee CK (1990) The removal of cationic dyes using coconut husk as an adsorbent. Pertanika 132:221–228Google Scholar
- Mahmoodi NM, Hayati B, Arami M, Lan C (2011) Adsorption of textile dyes on pine cone from colored wastewater: kinetic, equilibrium and thermodynamic studies. Desal 268:117–125Google Scholar
- Malik PK (2003) Use of activated carbons prepared from sawdust and rice-husk for adsorption of acidic dyes: a case study of acid yellow 36. Dyes Pigment 56:243–250Google Scholar
- Malik PK, Saha SK (2003) Oxidation of direct dyes with hydrogen peroxide using ferrous ion as catalyst. Sep Puri Technol 31:241–250Google Scholar
- Malik PK, Sanyal SK (2004) Kinetics of decolorization of azo dyes in wastewater by UV/H2O2 process. Sep Purif Technol 36:167–175Google Scholar
- Malik R, Ramteke DS, Wate SR (2007) Adsorption of Malachite green on groundnut shell waste based powdered activated carbon. Waste Manag 27:1129–1138Google Scholar
- Mall ID, Vimal CS, Nitin K (2006) Removal of Orange Green and Methyl violet dyes by adsorption on to bagasse flyash—kinetic study and equilibrium isotherm analysis. Dyes Pigment 69:210–223Google Scholar
- Manaskorn R, Ruangchua S, Teachakulwiroj S (2004) Removal of reactive dyes from aqueous solution using bagasse fly ash. Environ Hazard Manag 26:14–23Google Scholar
- Mane SM, Vanjara AK, Sawant MR (2005) Removal of Phenol from wastewater using date seed carbon. J Chin Chem Soc 526:1117–1122Google Scholar
- Marc R (1996) Asian textile dye makers are a growing power in changing market. C EN North East News Bureau 73:10–12Google Scholar
- Meng FW (2005) Study on a mathematical model in predicting breakthrough curves of fixed-bed adsorption onto resin adsorbent. MS Thesis, Nanjing University, China, pp 28–36Google Scholar
- Mishra G, Tripathy M (1993) A critical review of the treatment for decolorization of dye wastewater. Colourage 40:35–38Google Scholar
- Mittal A, Krishnan L, Gupta VK (2005) Removal and recovery of Malachite green from wastewater using an agricultural waste material, de-oiled soya. Sep Purif Technol 43:125–133Google Scholar
- Namasivayam C, Kavitha D (2002) Removal of Congo red from water by adsorption on to activated carbon prepared from coir pith, an agricultural solid waste. Dyes Pigment 54:47–58Google Scholar
- Namasivayam C, Muniasamy N, Gayathiri K, Rani M, Ranganathan K (1996) Removal of dyes from aqueous solution by cellulosic waste orange peel. Bioresour Technol 57:37–43Google Scholar
- Namasivayam C, Radhika R, Suba S (2001) Uptake of dyes by a promising locally available agricultural solid waste: coir pith. Waste Manag (Oxford) 21:381–387Google Scholar
- Neelavannan MG, Revathi M, Ahmed Basha C (2007) Photocatalytic and electro-chemical combined treatment of textile wastewater. J Hazard Mater 149:371–378Google Scholar
- Newcombe G, Drikas M (1997) Adsorption of NOM activated carbon: electrostatic and non-electrostatic effects. Carbon 35:1239–1250Google Scholar
- Ofomaja AE, Ho YS (2007) Equilibrium sorption of anionic dye from aqueous solution by palm kernel fibre as sorbent. Dyes Pigment 74:60–66Google Scholar
- Oladoja NA, Aboluwoye CO, Oladimeji YB (2008) Kinetics and isotherm studies on methylene blue adsorption onto ground palm kernel coat. Turkish J Eng Environ Sci 32:303–312Google Scholar
- Önal Y, Akmil-Basar C, Eren D, SarIcI-Özdemir Ç, Depci T (2006) Adsorption kinetics of Malachite green onto activated carbon prepared from Tunçbilek lignite. J Hazard Mater 128:150–157Google Scholar
- Ong ST, Keng PS, Lee CK (2010) Basic and reactive dyes sorption enhancement of rice hull through chemical modification. Am J Appl Sci 74:447–452Google Scholar
- Özcan A, Ömeroglu Ç, Erdogan Y, Özcan AS (2007) Modification of bentonite with a cationic surfactant: an adsorption study of textile dye Reactive Blue 19. J Hazard Mater 140:173–179Google Scholar
- Parab H, Suderesan M, Pathare N, Vaze B (2009) Use of agro-industrial wastes for removal of basic dyes from aqueous solutions. Clean 37:963–969Google Scholar
- Patel H, Vashi RT (2010) Adsorption of crystal violet dye onto tamarind seed powder. E-J Chem 73:975–984Google Scholar
- Pearce CI, Lloyd JR, Guthrie JT (2003) The removal of colour from textile wastewater using whole bacterial cells: a review. Dyes Pigment 58:179–196Google Scholar
- Ponnusami V, Vikiram S, Srivastava SN (2008) Guava Psidium guajava leaf powder: novel adsorbent for removal of methylene blue from aqueous solutions. J Hazard Maters 152:276–286Google Scholar
- Ponnusami V, Gunasekar V, Srivastava SN (2009) Kinetics of methylene blue removal from aqueous solution using gulmohar Delonix regia plant leaf powder: multivariate regression analysis. J Hazard Mater 169:119–127Google Scholar
- Qiu H, Lv L, Pan BC, Zhang QJ, Zhang WM, Zhang QX (2009) Critical review in adsorption kinetic models. J Zheijang Univ A 105:716–724Google Scholar
- Radovic LR, Silva IF, Ume JI, Menendez JA, Leon CA, Leon Y, Scaroni AW (1997) An experimental and theoretical study of the adsorption of aromatics possessing electron withdrawing and electron-donating functional groups by chemically modified activated carbons. Carbon 35:1339–1348Google Scholar
- Rajamohan N (2009) Equilibrium studies on sorption of an anionic dye onto acid activated water hyacinth roots. Afr J Environ Sci Technol 311:399–404Google Scholar
- Rajeswari S, Namasivayam C, Kadirvelu K (2001) Orange peel as an adsorbent in the removal of Acid violet 17 acid dye from aqueous solutions. Waste Manag 21:105–110Google Scholar
- Reichenberg D (1953) Properties of ion-exchange resin in relation to their structure. III. Kinetics of exchange. J Am Chem Soc 75:589Google Scholar
- Robinson T, Chandra B, Nigam P (2002a) Removal of dyes from a synthetic textile dye effluent by adsorption on apple pomace and wheat straw. Water Resour 36:2824–2830Google Scholar
- Robinson T, Chandran B, Nigam P (2002b) Studies on desorption of individual textile dyes and a synthetic dye effluent from dye adsorbed-agricultural residues using solvents. Bioresour Technol 84:299–301Google Scholar
- Robinson T, Chandran B, Sathya Naidu G, Nigam P (2002c) Studies on the removal of dyes from a synthetic textile effluent using barley husk in static-batch mode and in a continuous flow, packed-bed, reactor. Bioresour Technol 85:43Google Scholar
- Salleh MAM, Mahmoud DK, Karim WAWA, Idris A (2011) Cationic and anionic dye adsorption by agricultural solid wastes: a comprehensive review. Desali 280:1–13Google Scholar
- Savova D, Petrov N, Yardim MF, Ekinci E, Budinova T, Razvigorova M, Minkova V (2003) The influence of the texture and surface properties of carbon adsorbents obtained from biomass products on the adsorption of manganese ions from aqueous solution. Carbon 41:1897–1903Google Scholar
- Senthilkumaar S, Kalaamani P, Subburaam CV (2006) Liquid phase adsorption of crystal violet onto activated carbons derived from male flowers of coconut tree. J Hazard Mater 136:800–808Google Scholar
- Sharma YC, Uma S (2010) Optimization of parameters for adsorption of methylene blue on a low-cost activated carbon. J Chem Eng Data 55:435–439Google Scholar
- Shukla A, Zhang YH, Dubey P, Margrave JL, Shukla SS (2002) The role of sawdust in the removal of unwanted materials from water. J Hazard Mater B95:137–152Google Scholar
- Singh KP, Mohan D, Sinha S, Tondon GS, Gosh D (2003) Color removal from wastewater using low-cost activated carbon derived from agricultural waste material. Ind Eng Chem Resour 42:1965–1976Google Scholar
- Sivakumar P, Palanisamy N (2010) Mechanistic study of dye adsorption on to a novel non-conventional low-cost adsorbent. Adv Appl Sci Res 1(1):58–65Google Scholar
- Sohrabi MR, Ghavami M (2008) Photo catalytic degradation of Direct Red 23 dye using UV/TiO2: effect of operational parameters. J Hazard Mater 153:1235–1239Google Scholar
- Somasekhara Reddy MC (2006) Removal of direct dye from aqueous solution with an adsorbent made from tamarind fruit shell, an agricultural solid waste. J Ind Sci Res 65:443–446Google Scholar
- Sundarjanto G, Keller-Lehmann B, Keller J (2006) Optimization of integrated chemical-biological degradation of a reactive azo dye using response surface methodology. J Hazard Mater 138:160–168Google Scholar
- Tan IAMW, Hameed BH, Ahmad AL (2007) Equilibrium and kinetic studies on basic dye adsorption by oil palm fibre activated carbon. Chem Eng J 127:111–119Google Scholar
- Tanyildizi MS (2011) Modeling of adsorption isotherms and kinetics of reactive dye from aqueous solution by peanut hull. Chem Eng J 168:1234–1240Google Scholar
- Teles de Vasconcelos LA, Gonzalez Beca CG (1993) Adsorption equilibria between pine bark and several ions in aqueous solution CdII, CrIII and HgII. Eur Water Poll Control 3:29–39Google Scholar
- Thinakaran N, Panneerselvam P, Baskaralingam P, Pulikesi M, Sivanesan S (2008) Removal of acid violet 17 from aqueous solutions by adsorption onto activated carbon prepared from sunflower seed hull. J Hazard Mater 154:204–212Google Scholar
- Venckatesh R, Amudha T, Sivaraj R, Chandramohan M, Jambulingam M (2010) Kinetics and equilibrium studies of adsorption of Direct Red-28 onto Punica granatum carbon. Inter J Eng Sci Technol 26:2040–2050Google Scholar
- Wang XS, Qin Y (2005) Equilibrium sorption isotherms for of Cu2+ on rice bran. Process Biochem 40:677–680Google Scholar
- Wang S, Li H, Xie S, Li S, Xu L (2006) Physical and chemical regeneration of zeolitic adsorbents for dye removal in wastewater treatment. Chemosphere 65:82–87Google Scholar
- Wang XU, Zhou Y, Jiang Y, Sun C (2008) The removal of basic dyes from aqueous solutions using agricultural by-products. J Hazard Mater 157:374–385Google Scholar
- Waranusantigul P, Pokethitiyook P, Kruatrachue M, Upatham ES (2003) Kinetics of basic dye methylene blue biosorption by giant duck week Spirodela polyrrhiza. Environ Poll 385:92Google Scholar
- Weber TW, Chakkravorti RK (1974) Pore and solid diffusion models for fixed-bed adsorbers. Am Inst Chem Eng J 20:228Google Scholar
- Weber WJ, Morris JC (1963) Kinetics of adsorption on carbon from solution. J Sanit Eng Divi 89(31):312Google Scholar
- Weng CH, Lin YT, Tzeng TW (2009) Removal of methylene blue from aqueous solution by adsorption onto pineapple leaf powder. J Hazard Mater 170:417–424Google Scholar
- Zawani Z, Luqman Chuah A, Choong TSY (2009) Equilibrium, kinetics and thermodynamic studies: adsorption of Remazol Black 5 on the palm kernel shell activated carbon PKS-AC. Eur J Sci Res 37:67–76Google Scholar
- Zeldowitsch J (1934) Über den mechanismus der katalytischen oxidation on CO and MnO2. Acta Physicochim URSS 1364–449Google Scholar
This article is published under license to BioMed Central Ltd. Open AccessThis article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.